Sensing and Bio-Sensing Research 5 (2015) 71–77
brought to you by COREView metadata, citation and similar papers at core.ac.uk
provided by Elsevier - Publisher Connector
Contents lists available at ScienceDirect
Sensing and Bio-Sensing Research
journal homepage: www.elsevier .com/locate /sbsr
Fabrication of multianalyte CeO2 nanograin electrolyte–insulator–
semiconductor biosensors by using CF4 plasma treatment
2214-1804/� 2015 The Authors. Published by Elsevier B.V.
This is an open access article under the CC BY-NC-ND license (http://creativecommons.org/licenses/by-nc-nd/4.0/).
⇑ Corresponding author.
E-mail addresses: firstname.lastname@example.org, email@example.com (H. Chen).
Chyuan Haur Kao a,d, Hsiang Chen b,⇑, Fang Yao Stephen Hou c, Shan Wei Chang a,d, Che Wei Chang a,d,
Chao Sung Lai a,d, Chin Pang Chen b, Yun Yang He b, Shang-Ren Lin b, Kun Min Hsieh b, Min Han Lin b
a Department of Electronic Engineering, Chang Gung University, Taiwan, ROC
b Department of Applied Materials and Optoelectronic Engineering, National Chi Nan University, Taiwan, ROC
c Clinical Laboratory, Marquette University, USA
d Center for Biomedical Engineering, Chang Gung University, Taiwan, ROC
a r t i c l e i n f o a b s t r a c t
Received 16 April 2015
Revised 27 June 2015
Accepted 1 July 2015
CF4 plasma treatment
Multianalyte CeO2 biosensors have been demonstrated to detect pH, glucose, and urine concentrations.
To enhance the multianalyte sensing capability of these biosensors, CF4 plasma treatment was applied
to create nanograin structures on the CeO2 membrane surface and thereby increase the contact surface
area. Multiple material analyses indicated that crystallization or grainization caused by the incorporation
of flourine atoms during plasma treatment might be related to the formation of the nanograins. Because
of the changes in surface morphology and crystalline structures, the multianalyte sensing performance
was considerably enhanced. Multianalyte CeO2 nanograin electrolyte–insulator–semiconductor biosen-
sors exhibit potential for use in future biomedical sensing device applications.
� 2015 The Authors. Published by Elsevier B.V. This is an open access article under the CC BY-NC-ND
Over the past 10 years nanostructure-based biosensors have
been intensively studied because of their distinct sensing capabil-
ity [1,2]. It is commonly acknowledged that the biosensing proper-
ties of these sensors are not only relevant to their dimensions but
also to their shapes [3–5]. Therefore, managing the morphologies
of sensing membranes is a crucial and an efficient approach to
acquiring preferable features [6,7]. Shape-controlled fabrication
processes have been demonstrated, and nanostructures with vari-
ous shapes such as cubes, wires, and rods have been designed
using various synthesis techniques [8–10]. Because the surface
contact area of a membrane can be enlarged and the number of
the surface sites can be increased, biosensors with desirable mor-
phologies can achieve high sensitivity and linearity [11,12].
Recently, EIS structures have been intensively investigated because
of their simple structure and fast detection [13,14]. To enhance
multianalyte sensing performance, various materials, alternative
processes, and treatments such as annealing have been incorpo-
rated [15,16]. However, multianalyte biosensing EIS membranes
with nanostructures on the membrane have not yet been clearly
reported. In this research, we introduced CF4 plasma treatment
to shape nanostructures and, thus, increase the surface area and
the number of surface sites of the membrane . Nanograin
structures formed using plasma treatment were observed in
atomic force microscope (AFM) and scanning electron microscope
(SEM) images . Secondary ion mass spectroscopy (SIMS) results
indicated that fluorine atoms on the membrane surface might be
related to the formation of nanostructures. Consistent with the
AFM and SEM images, X-ray diffraction (XRD) patterns and X-ray
photoelectron spectroscopy (XPS) measurements confirmed that
crystallization and grainization of CeO2 might cause the formation
of nanostructures . The CeO2 multianalyte biosensor demon-
strated multiple sensing capability with solutions containing
H+, Na+, K+, glucose , and urea . Furthermore, the results
indicated that the formation of nanograins on the CeO2 membrane
further enhanced the multianalyte sensing capability of various
The impact of the development of nanograins on the under-
standing of the detecting film can be illustrated by considering
the site-binding design in an explanation of the ionic consumption
procedures at the electrolyte/oxide interface . For pH detecting
ability, the reaction voltage relies on the outer lining area prospec-
tive (w), which is an operation of the membrane content and the
pH of the electrolyte [13,22]. The value of (w) can be calculated
using Eq. (2).
Fig. 1. FESEM images of the CeO2 film (a) before and (b) after CF4 plasma treatment for 15 s. AFM images of the CeO2 film (c) before and (d) after CF4 plasma treatment for
Fig. 2. SIMS profiles for the CeO2 film treated with CF4 plasma for 15 s.
72 C.H. Kao et al. / Sensing and Bio-Sensing Research 5 (2015) 71–77
The influence of the formation of nanograins on the detection of
the sensing film can be understood by considering the site-binding
model. To illustrate the ionic absorption procedures at the
electrolyte/oxide interface involved in pH sensing, the detecting
voltage on the surface potential (w) can be expressed as a function
of the membrane material and the pH value of the electrolyte. The
value of (w) can be calculated using Eq. (1).
w ¼ 2:303 kT
bþ 1 ðpHpzc � pHÞ ð1Þ
where k is Boltzmann’s constant, T is the temperature, q is the ele-
mentary charge, pHpzc is the pH value with zero charge, and b is a
factor that signifies the chemical sensitivity of the gate oxide.
Furthermore, the b value is proportional to the chemical sensitivity
of the gate dielectric and is determined according to the density of
surface hydroxyl groups, as described in Eq. (2).
b ¼ 2q
where Ns is the count of surface site per unit area and CDL is the
double layer capacitance based on the Gouy–Chapman–Stern model
. According to Eqs. (1) and (2), a can be expected to result in a
higher sensitivity and linearity in accordance with the value
revealed in the report . Nanograins formed through plasma
treatment can noticeably increase the surface area and, hence, the
surface sites; therefore, the sensing performance can be enhanced
by incorporating plasma treatment.
2. Experimental details
EIS biosensors containing CeO2 membranes were designed on
4-inch n-type (100) Si wafers with a resistivity of 5–10 X-cm.
After RCA cleaning procedure, the wafers were dropped into 1%
hydrofluoric acid to eliminate oxide from the surface. First, a
50-nm CeO2 membrane was placed on the Si substrate through
radio frequency (rf) sputtering from a cerium target in a diluted
O2 ambient (Ar/O2 = 20 sccm/5 sccm). The rf power and ambient
pressure were 100 W and 20 mTorr, respectively. After deposition,
CeO2 membrane layers were subjected to a post-CF4 treatment in a
plasma-enhanced chemical vapor deposition system with an rf
power of 30 W and a processing pressure of 500 mTorr for 15,
30, and 60 s, respectively. Subsequently, the back-side contact of
the Si wafer was grown using a 300-nm Al film. The size of the
sensing membrane was defined through photolithographic pro-
cessing under a photosensitive epoxy (SU8-2005, Micro-Chem).
EIS structures were then placed on the copper lines of a printed cir-
cuit board by using a silver gel. An epoxy package was included to
separate the EIS structure and the copper line. The device structure
is shown in the supplement data.